#------------------------------------------------------------------------------
#$Date: 2023-08-05 19:38:36 +0300 (Sat, 05 Aug 2023) $
#$Revision: 285553 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/96/1569636.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1569636
loop_
_publ_author_name
'Smirnova, Ekaterina S.'
'Alekseeva, Olga A.'
'Artemov, Vladimir V.'
'Sorokin, Timofei A.'
'Khmelenin, Dmitry N.'
'Sidorova, Ekaterina V.'
'Frolov, Kirill V.'
'Gudim, Irina A.'
_publ_section_title
;
 Crystal Structure of Bismuth-Containing Samarium Iron--Aluminium Borates
 Sm1−xBixFe3−yAly(BO3)4 (x = 0.05--0.07, y = 0--0.28) in the
 Temperature Range of 25--500 K
;
_journal_issue                   7
_journal_name_full               Crystals
_journal_page_first              1128
_journal_paper_doi               10.3390/cryst13071128
_journal_volume                  13
_journal_year                    2023
_chemical_formula_sum            'Al0.07 B4 Bi0.07 Fe2.93 O12 Sm0.93'
_chemical_formula_weight         555.2
_space_group_IT_number           155
_space_group_name_Hall           'R 3 2"'
_space_group_name_H-M_alt        'R 3 2 :H'
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      155
_symmetry_space_group_name_Hall  'R 3 2"'
_symmetry_space_group_name_H-M   'R 3 2 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   9.55950(10)
_cell_length_b                   9.55950(10)
_cell_length_c                   7.58160(10)
_cell_measurement_reflns_used    18047
_cell_measurement_temperature    292.98(14)
_cell_measurement_theta_max      73.91
_cell_measurement_theta_min      4.25
_cell_volume                     600.015(12)
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_diffrn_ambient_temperature      293
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1745
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.97
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, EosS2 with high theta cut'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0265
_diffrn_reflns_av_unetI/netI     0.0141
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            20709
_diffrn_reflns_theta_full        65.49
_diffrn_reflns_theta_max         74.37
_diffrn_reflns_theta_min         3.64
_diffrn_source                   'fine-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    13.558
_exptl_absorpt_correction_T_max  0.1913
_exptl_absorpt_correction_T_min  0.091
_exptl_absorpt_correction_type   sphere
_exptl_absorpt_process_details   Jana2006
_exptl_crystal_colour            light-green
_exptl_crystal_density_diffrn    4.6096
_exptl_crystal_description       Sphere
_exptl_crystal_F_000             770
_exptl_crystal_size_rad          0.12
_refine_diff_density_max         0.79
_refine_diff_density_min         -0.90
_refine_ls_abs_structure_details
'  1220 of Friedel pairs used in the refinement'
_refine_ls_abs_structure_Flack   0.900(4)
_refine_ls_extinction_coef       2340(50)
_refine_ls_extinction_method
'B-C type 1 Lorentzian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.01
_refine_ls_goodness_of_fit_ref   1.01
_refine_ls_number_constraints    7
_refine_ls_number_parameters     36
_refine_ls_number_reflns         2697
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0115
_refine_ls_R_factor_gt           0.0115
_refine_ls_shift/su_max          0.0458
_refine_ls_shift/su_mean         0.0092
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0151
_refine_ls_wR_factor_ref         0.0151
_reflns_number_gt                2696
_reflns_number_total             2697
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            S2-SmFe_Al05.cif
_cod_data_source_block           Al05
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/current/MDPI/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_exptl_absorpt_correction_type' value 'Sphere' was changed
to 'sphere' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/current/MDPI/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 
;
_cod_original_sg_symbol_H-M      'R 3 2'
_cod_database_code               1569636
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 y,x,-z
5 x-y,-y,-z
6 -x,-x+y,-z
7 x+2/3,y+1/3,z+1/3
8 -y+2/3,x-y+1/3,z+1/3
9 -x+y+2/3,-x+1/3,z+1/3
10 y+2/3,x+1/3,-z+1/3
11 x-y+2/3,-y+1/3,-z+1/3
12 -x+2/3,-x+y+1/3,-z+1/3
13 x+1/3,y+2/3,z+2/3
14 -y+1/3,x-y+2/3,z+2/3
15 -x+y+1/3,-x+2/3,z+2/3
16 y+1/3,x+2/3,-z+2/3
17 x-y+1/3,-y+2/3,-z+2/3
18 -x+1/3,-x+y+2/3,-z+2/3
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0 0 0 Uani 0.007748(11) 3 0.93 d . . .
Bi1 Bi 0 0 0 Uani 0.007748(11) 3 0.07 d . . .
Fe1 Fe 0.217034(11) 0.333333 0.333333 Uani 0.005268(18) 9 0.9767 d . . .
Al1 Al 0.217034(11) 0.333333 0.333333 Uani 0.005268(18) 9 0.0233 d . . .
O1 O 0.14435(5) 0.14435(5) 0.5 Uani 0.00694(8) 9 1 d . . .
O2 O 0.40944(7) 0.40944(7) 0.5 Uani 0.01150(12) 9 1 d . . .
O3 O 0.02597(5) 0.21377(6) 0.18382(7) Uani 0.00843(8) 18 1 d . . .
B1 B 0 0 0.5 Uani 0.00563(16) 3 1 d . . .
B2 B 0.55312(8) 0.55312(8) 0.5 Uani 0.00642(14) 9 1 d . . .
loop_
_atom_site_aniso_label
_atom_site_aniso_type_symbol
_atom_site_aniso_U_11
_atom_site_aniso_U_22
_atom_site_aniso_U_33
_atom_site_aniso_U_12
_atom_site_aniso_U_13
_atom_site_aniso_U_23
Sm1 Sm 0.007981(13) 0.007981(13) 0.00728(2) 0.003991(6) 0 0
Bi1 Bi 0.007981(13) 0.007981(13) 0.00728(2) 0.003991(6) 0 0
Fe1 Fe 0.004998(18) 0.00510(2) 0.00574(4) 0.002550(11) -0.000059(8)
-0.000119(15)
Al1 Al 0.004998(18) 0.00510(2) 0.00574(4) 0.002550(11) -0.000059(8)
-0.000119(15)
O1 O 0.00515(7) 0.00515(7) 0.00879(17) 0.00128(8) -0.00097(5) 0.00097(5)
O2 O 0.00690(9) 0.00690(9) 0.0159(3) -0.00014(12) -0.00420(10) 0.00420(10)
O3 O 0.00618(8) 0.01009(11) 0.00953(13) 0.00445(8) -0.00144(8) -0.00182(9)
B1 B 0.00497(16) 0.00497(16) 0.0069(4) 0.00249(8) 0 0
B2 B 0.00545(13) 0.00545(13) 0.0080(2) 0.00242(19) -0.00021(10) 0.00021(10)
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al 0.0645 0.0514 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
B 0.0013 0.0007 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Bi -4.1077 10.2566 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Fe 0.3463 0.8444 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sm -0.1638 3.4418 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Bi1 Sm1 O3 . . . 0 ?
Bi1 Sm1 O3 . . 2_555 0 ?
Bi1 Sm1 O3 . . 3_555 0 ?
Bi1 Sm1 O3 . . 4_555 0 ?
Bi1 Sm1 O3 . . 5_555 0 ?
Bi1 Sm1 O3 . . 6_555 0 ?
O3 Sm1 O3 . . 2_555 89.222(19) ?
O3 Sm1 O3 . . 3_555 89.222(19) ?
O3 Sm1 O3 . . 4_555 122.483(14) ?
O3 Sm1 O3 . . 5_555 142.10(2) ?
O3 Sm1 O3 . . 6_555 72.61(2) ?
O3 Sm1 O3 2_555 . 3_555 89.222(19) ?
O3 Sm1 O3 2_555 . 4_555 142.10(2) ?
O3 Sm1 O3 2_555 . 5_555 72.606(18) ?
O3 Sm1 O3 2_555 . 6_555 122.48(2) ?
O3 Sm1 O3 3_555 . 4_555 72.61(2) ?
O3 Sm1 O3 3_555 . 5_555 122.48(2) ?
O3 Sm1 O3 3_555 . 6_555 142.096(13) ?
O3 Sm1 O3 4_555 . 5_555 89.222(19) ?
O3 Sm1 O3 4_555 . 6_555 89.222(19) ?
O3 Sm1 O3 5_555 . 6_555 89.222(19) ?
Sm1 Bi1 O3 . . . 0 ?
Sm1 Bi1 O3 . . 2_555 0 ?
Sm1 Bi1 O3 . . 3_555 0 ?
Sm1 Bi1 O3 . . 4_555 0 ?
Sm1 Bi1 O3 . . 5_555 0 ?
Sm1 Bi1 O3 . . 6_555 0 ?
O3 Bi1 O3 . . 2_555 89.222(19) ?
O3 Bi1 O3 . . 3_555 89.222(19) ?
O3 Bi1 O3 . . 4_555 122.483(14) ?
O3 Bi1 O3 . . 5_555 142.10(2) ?
O3 Bi1 O3 . . 6_555 72.61(2) ?
O3 Bi1 O3 2_555 . 3_555 89.222(19) ?
O3 Bi1 O3 2_555 . 4_555 142.10(2) ?
O3 Bi1 O3 2_555 . 5_555 72.606(18) ?
O3 Bi1 O3 2_555 . 6_555 122.48(2) ?
O3 Bi1 O3 3_555 . 4_555 72.61(2) ?
O3 Bi1 O3 3_555 . 5_555 122.48(2) ?
O3 Bi1 O3 3_555 . 6_555 142.096(13) ?
O3 Bi1 O3 4_555 . 5_555 89.222(19) ?
O3 Bi1 O3 4_555 . 6_555 89.222(19) ?
O3 Bi1 O3 5_555 . 6_555 89.222(19) ?
Al1 Fe1 O1 . . . 0 ?
Al1 Fe1 O1 . . 15_554 0 ?
Al1 Fe1 O2 . . . 0 ?
Al1 Fe1 O2 . . 15_554 0 ?
Al1 Fe1 O3 . . . 0 ?
Al1 Fe1 O3 . . 17_555 0 ?
O1 Fe1 O1 . . 15_554 168.17(3) ?
O1 Fe1 O2 . . . 77.148(17) ?
O1 Fe1 O2 . . 15_554 94.21(2) ?
O1 Fe1 O3 . . . 92.102(18) ?
O1 Fe1 O3 . . 17_555 95.47(2) ?
O1 Fe1 O2 15_554 . . 94.213(19) ?
O1 Fe1 O2 15_554 . 15_554 77.15(2) ?
O1 Fe1 O3 15_554 . . 95.47(2) ?
O1 Fe1 O3 15_554 . 17_555 92.10(2) ?
O2 Fe1 O2 . . 15_554 87.48(3) ?
O2 Fe1 O3 . . . 167.55(3) ?
O2 Fe1 O3 . . 17_555 87.07(3) ?
O2 Fe1 O3 15_554 . . 87.08(2) ?
O2 Fe1 O3 15_554 . 17_555 167.55(2) ?
O3 Fe1 O3 . . 17_555 100.35(3) ?
Fe1 O1 Fe1 . . 8_555 103.572(17) ?
Fe1 O1 B1 . . . 128.21(2) ?
Fe1 O1 B1 8_555 . . 128.21(2) ?
Fe1 O2 Fe1 . . 8_555 102.13(2) ?
Fe1 O2 B2 . . . 128.93(4) ?
Fe1 O2 B2 8_555 . . 128.93(4) ?
Sm1 O3 Bi1 . . . 0.0(5) ?
Sm1 O3 Fe1 . . . 120.39(3) ?
Sm1 O3 B2 . . 13_444 107.13(3) ?
Bi1 O3 Fe1 . . . 120.39(3) ?
Bi1 O3 B2 . . 13_444 107.13(3) ?
Fe1 O3 B2 . . 13_444 132.35(4) ?
O1 B1 O1 . . 2_555 120.00(4) ?
O1 B1 O1 . . 3_555 120.00(4) ?
O1 B1 O1 2_555 . 3_555 120.00(4) ?
O2 B2 O3 . . 7_555 117.77(7) ?
O2 B2 O3 . . 16_555 117.77(7) ?
O3 B2 O3 7_555 . 16_555 124.46(5) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sm1 Bi1 . . 0 ?
Sm1 O3 . . 2.3817(6) ?
Sm1 O3 . 2_555 2.3817(5) ?
Sm1 O3 . 3_555 2.3817(7) ?
Sm1 O3 . 4_555 2.3817(6) ?
Sm1 O3 . 5_555 2.3817(5) ?
Sm1 O3 . 6_555 2.3817(7) ?
Bi1 O3 . . 2.3817(6) ?
Bi1 O3 . 2_555 2.3817(5) ?
Bi1 O3 . 3_555 2.3817(7) ?
Bi1 O3 . 4_555 2.3817(6) ?
Bi1 O3 . 5_555 2.3817(5) ?
Bi1 O3 . 6_555 2.3817(7) ?
Fe1 Al1 . . 0 ?
Fe1 O1 . . 2.0219(4) ?
Fe1 O1 . 15_554 2.0219(3) ?
Fe1 O2 . . 2.0423(5) ?
Fe1 O2 . 15_554 2.0423(8) ?
Fe1 O3 . . 1.9595(4) ?
Fe1 O3 . 17_555 1.9596(7) ?
O1 B1 . . 1.3799(4) ?
O2 B2 . . 1.3735(7) ?
O3 B2 . 13_444 1.3695(10) ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?
loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?
loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?
loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.100(4) 1 0 0 0 1 0 0 0 1
2 0.900(4) -1 0 0 0 -1 0 0 0 -1
loop_
_jana_atom_site_adp_c_label
_jana_atom_site_adp_c_type_symbol
_jana_atom_site_adp_c_111
_jana_atom_site_adp_c_112
_jana_atom_site_adp_c_113
_jana_atom_site_adp_c_122
_jana_atom_site_adp_c_123
_jana_atom_site_adp_c_133
_jana_atom_site_adp_c_222
_jana_atom_site_adp_c_223
_jana_atom_site_adp_c_233
_jana_atom_site_adp_c_333
? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_d_label
_jana_atom_site_adp_d_type_symbol
_jana_atom_site_adp_d_1111
_jana_atom_site_adp_d_1112
_jana_atom_site_adp_d_1113
_jana_atom_site_adp_d_1122
_jana_atom_site_adp_d_1123
_jana_atom_site_adp_d_1133
_jana_atom_site_adp_d_1222
_jana_atom_site_adp_d_1223
_jana_atom_site_adp_d_1233
_jana_atom_site_adp_d_1333
_jana_atom_site_adp_d_2222
_jana_atom_site_adp_d_2223
_jana_atom_site_adp_d_2233
_jana_atom_site_adp_d_2333
_jana_atom_site_adp_d_3333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_e_label
_jana_atom_site_adp_e_type_symbol
_jana_atom_site_adp_e_11111
_jana_atom_site_adp_e_11112
_jana_atom_site_adp_e_11113
_jana_atom_site_adp_e_11122
_jana_atom_site_adp_e_11123
_jana_atom_site_adp_e_11133
_jana_atom_site_adp_e_11222
_jana_atom_site_adp_e_11223
_jana_atom_site_adp_e_11233
_jana_atom_site_adp_e_11333
_jana_atom_site_adp_e_12222
_jana_atom_site_adp_e_12223
_jana_atom_site_adp_e_12233
_jana_atom_site_adp_e_12333
_jana_atom_site_adp_e_13333
_jana_atom_site_adp_e_22222
_jana_atom_site_adp_e_22223
_jana_atom_site_adp_e_22233
_jana_atom_site_adp_e_22333
_jana_atom_site_adp_e_23333
_jana_atom_site_adp_e_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
loop_
_jana_atom_site_adp_f_label
_jana_atom_site_adp_f_type_symbol
_jana_atom_site_adp_f_111111
_jana_atom_site_adp_f_111112
_jana_atom_site_adp_f_111113
_jana_atom_site_adp_f_111122
_jana_atom_site_adp_f_111123
_jana_atom_site_adp_f_111133
_jana_atom_site_adp_f_111222
_jana_atom_site_adp_f_111223
_jana_atom_site_adp_f_111233
_jana_atom_site_adp_f_111333
_jana_atom_site_adp_f_112222
_jana_atom_site_adp_f_112223
_jana_atom_site_adp_f_112233
_jana_atom_site_adp_f_112333
_jana_atom_site_adp_f_113333
_jana_atom_site_adp_f_122222
_jana_atom_site_adp_f_122223
_jana_atom_site_adp_f_122233
_jana_atom_site_adp_f_122333
_jana_atom_site_adp_f_123333
_jana_atom_site_adp_f_133333
_jana_atom_site_adp_f_222222
_jana_atom_site_adp_f_222223
_jana_atom_site_adp_f_222233
_jana_atom_site_adp_f_222333
_jana_atom_site_adp_f_223333
_jana_atom_site_adp_f_233333
_jana_atom_site_adp_f_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?
